Double Spin Crossovers: A New Double Salt Strategy to Improve Magnetic and Memory Properties
Murray, Keith S.; Phonsri, Wasinee; Jameson, Guy N. L.; Lewis, Barnaby; Chemical Communications  (2019) –; doi:10.1039/C9CC07416C

data_7124391
_publ_section_title
;
 Double Spin Crossovers: A New Double Salt Strategy to Improve Magnetic
 and Memory Properties
;
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/C9CC07416C
_journal_year                    2019
_chemical_formula_moiety
'C26 H32 Fe N12, C24 H16 Fe N4 O4, Cl O4, 2(C2 H3 N)'
_chemical_formula_sum            'C54 H54 Cl Fe2 N18 O8'
_chemical_formula_weight         1230.30
_chemical_name_common            '[Fe(3,5 Me2TPM)(TPM)][Fe(azp)2]ClO4 2MeCN'
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2019-05-22 deposited with the CCDC.    2019-10-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 100.41(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   16.948(3)
_cell_length_b                   10.425(2)
_cell_length_c                   31.438(6)
_cell_measurement_reflns_used    15449
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      31.814
_cell_measurement_theta_min      0.789
_cell_volume                     5463.1(18)
_computing_cell_refinement       'XDS (Kabsch, 1993)'
_computing_data_collection       'BluIce (McPhillips, 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    X-SEED
_computing_publication_material  'XCIF V6.12 (BrukerAXS, 2001).'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.963
_diffrn_measured_fraction_theta_max 0.788
_diffrn_measurement_device_type  'ADSC Quantum 210r'
_diffrn_measurement_method       'Phi Scan'
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0338
_diffrn_reflns_av_unetI/netI     0.0204
_diffrn_reflns_Laue_measured_fraction_full 0.963
_diffrn_reflns_Laue_measured_fraction_max 0.788
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       46
_diffrn_reflns_limit_l_min       -46
_diffrn_reflns_number            89605
_diffrn_reflns_point_group_measured_fraction_full 0.963
_diffrn_reflns_point_group_measured_fraction_max 0.788
_diffrn_reflns_theta_full        27.500
_diffrn_reflns_theta_max         31.814
_diffrn_reflns_theta_min         1.952
_diffrn_source                   'MX1, Australian Synchrotron'
_exptl_absorpt_coefficient_mu    0.653
_exptl_absorpt_correction_T_max  0.993
_exptl_absorpt_correction_T_min  0.977
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'XScale within XDS'
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    1.496
_exptl_crystal_description       Plate
_exptl_crystal_F_000             2548
_exptl_crystal_preparation       'Magnetic properties'
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.010
_refine_diff_density_max         0.559
_refine_diff_density_min         -0.943
_refine_diff_density_rms         0.083
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.054
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     794
_refine_ls_number_reflns         14724
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.054
_refine_ls_R_factor_all          0.0487
_refine_ls_R_factor_gt           0.0445
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0599P)^2^+6.2393P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1186
_refine_ls_wR_factor_ref         0.1211
_reflns_Friedel_coverage         0.000
_reflns_number_gt                13449
_reflns_number_total             14724
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9cc07416c2.cif
_cod_data_source_block           WS283_b
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-Scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        5463(2)
_cod_database_code               7124391
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.968
_shelx_estimated_absorpt_t_max   0.993
_shelx_res_checksum              70717